  The Pariser-Parr-Pople Hamiltonian is used to calculate and identify the
nature of the low-lying vertical transition energies of polydiacetylene. The
model is solved using the density matrix renormalisation group method for a
fixed acetylenic geometry for chains of up to 102 atoms. The non-linear optical
properties of polydiacetylene are considered, which are determined by the
third-order susceptibility. The experimental 1Bu data of Giesa and Schultz are
used as the geometric model for the calculation. For short chains, the
calculated E(1Bu) agrees with the experimental value, within solvation effects
(ca. 0.3 eV). The charge gap is used to characterise bound and unbound states.
The nBu is above the charge gap and hence a continuum state; the 1Bu, 2Ag and
mAg are not and hence are bound excitons. For large chain lengths, the nBu
tends towards the charge gap as expected, strongly suggesting that the nBu is
the conduction band edge. The conduction band edge for PDA is agreed in the
literature to be ca. 3.0 eV. Accounting for the strong polarisation effects of
the medium and polaron formation gives our calculated E(nBu) ca. 3.6 eV, with
an exciton binding energy of ca. 1.0 eV. The 2Ag state is found to be above the
1Bu, which does not agree with relaxed transition experimental data. However,
this could be resolved by including explicit lattice relaxation in the Pariser-
Parr-Pople-Peierls model. Particle-hole separation data further suggest that
the 1Bu, 2Ag and mAg are bound excitons, and that the nBu is an unbound
exciton.
